# chapter 6: diffusion in solids

Post on 16-Mar-2016

69 views

Embed Size (px)

DESCRIPTION

CHAPTER 6: DIFFUSION IN SOLIDS. ISSUES TO ADDRESS. • How does diffusion occur?. • Why is it an important part of processing?. • How can the rate of diffusion be predicted for some simple cases?. • How does diffusion depend on structure and temperature?. 1. DIFFUSION DEMO. - PowerPoint PPT PresentationTRANSCRIPT

ISSUES TO ADDRESS... How does diffusion occur? Why is it an important part of processing? How can the rate of diffusion be predicted for some simple cases?1 How does diffusion depend on structure and temperature?CHAPTER 6:DIFFUSION IN SOLIDS

2 Glass tube filled with water. At time t = 0, add some drops of ink to one end of the tube. Measure the diffusion distance, x, over some time. Compare the results with theory.DIFFUSION DEMO

3 Interdiffusion: In an alloy, atoms tend to migrate from regions of large concentration.InitiallyAfter some timeAdapted from Figs. 5.1 and 5.2, Callister 6e.DIFFUSION: THE PHENOMENA (1)

4 Self-diffusion: In an elemental solid, atoms also migrate.Label some atomsAfter some timeDIFFUSION: THE PHENOMENA (2)

5Substitutional Diffusion: applies to substitutional impurities atoms exchange with vacancies rate depends on: --number of vacancies --activation energy to exchange.DIFFUSION MECHANISMS

6 Simulation of interdiffusion across an interface: Rate of substitutional diffusion depends on: --vacancy concentration --frequency of jumping.(Courtesy P.M. Anderson)DIFFUSION SIMULATIONClick on image to animate

7(Courtesy P.M. Anderson) Applies to interstitial impurities. More rapid than vacancy diffusion. Simulation: --shows the jumping of a smaller atom (gray) from one interstitial site to another in a BCC structure. The interstitial sites considered here are at midpoints along the unit cell edges.INTERSTITIAL SIMULATIONClick on image to animate

Case Hardening: --Diffuse carbon atoms into the host iron atoms at the surface. --Example of interstitial diffusion is a case hardened gear. Result: The "Case" is --hard to deform: C atoms "lock" planes from shearing. --hard to crack: C atoms put the surface in compression.8Fig. 5.0, Callister 6e.(Fig. 5.0 iscourtesy ofSurface Division, Midland-Ross.)PROCESSING USING DIFFUSION (1)

Doping Silicon with P for n-type semiconductors: Process:91. Deposit P rich layers on surface.2. Heat it.3. Result: Doped semiconductor regions.Fig. 18.0, Callister 6e.PROCESSING USING DIFFUSION (2)

Flux:10 Directional Quantity Flux can be measured for: --vacancies --host (A) atoms --impurity (B) atomsMODELING DIFFUSION: FLUX

Concentration Profile, C(x): [kg/m3]11 Fick's First Law: The steeper the concentration profile, the greater the flux!Adapted from Fig. 5.2(c), Callister 6e.CONCENTRATION PROFILES & FLUX

Steady State: the concentration profile doesn't change with time.12 Apply Fick's First Law: Result: the slope, dC/dx, must be constant (i.e., slope doesn't vary with position)! If Jx)left = Jx)right , thenSTEADY STATE DIFFUSION

Steel plate at 700C with geometry shown:13 Q: How much carbon transfers from the rich to the deficient side?Adapted from Fig. 5.4, Callister 6e.EX: STEADY STATE DIFFUSION

Concentration profile, C(x), changes w/ time.14 To conserve matter: Fick's First Law: Governing Eqn.:NON STEADY STATE DIFFUSION

Copper diffuses into a bar of aluminum.15 General solution:"error function"Values calibrated in Table 5.1, Callister 6e. Adapted from Fig. 5.5, Callister 6e.EX: NON STEADY STATE DIFFUSION

Copper diffuses into a bar of aluminum. 10 hours at 600C gives desired C(x). How many hours would it take to get the same C(x) if we processed at 500C?16 Result: Dt should be held constant. Answer:Note: valuesof D areprovided here.Key point 1: C(x,t500C) = C(x,t600C).Key point 2: Both cases have the same Co and Cs.PROCESSING QUESTION

17 The experiment: we recorded combinations of t and x that kept C constant. Diffusion depth given by:= (constant here)DIFFUSION DEMO: ANALYSIS

Experimental result: x ~ t0.58 Theory predicts x ~ t0.50 Reasonable agreement!18DATA FROM DIFFUSION DEMO

Diffusivity increases with T. Experimental Data:D has exp. dependence on TRecall: Vacancy does also!19Adapted from Fig. 5.7, Callister 6e. (Date for Fig. 5.7 taken from E.A. Brandes and G.B. Brook (Ed.) Smithells Metals Reference Book, 7th ed., Butterworth-Heinemann, Oxford, 1992.)DIFFUSION AND TEMPERATURE

20Diffusion FASTER for...

open crystal structures

lower melting T materials

materials w/secondary bonding

smaller diffusing atoms

cations

lower density materialsDiffusion SLOWER for...

close-packed structures

higher melting T materials

materials w/covalent bonding

larger diffusing atoms

anions

higher density materialsSUMMARY:STRUCTURE & DIFFUSION

Reading:Core Problems:Self-help Problems:0ANNOUNCEMENTS

Typically, we let the experiment described on slide 2 run during the class; at this point in the class, the results are available for the class to look at.